American Journal of Engineering Research (AJER)
201
3
w w w.a j e r.u s
w w w.a j e r.u s
Page
67
Page
67
American Journal of Engineering Research (AJER)
e

ISSN: 2320

0847 p

ISSN : 2320

0936
Volume

2, Issue

4, pp

67

71
www.ajer.us
Research Paper
Open Access
Evaluation
of Relationship
Between Mechanical
Properties
o
f
High Strength Self Compacting Concrete
S.SeshaPhani
1
,Dr.Seshadri Sekhar T
2
,
Dr.Srinivasa Rao
3,
Dr Sravana
4
1
Deputy Executive
Engineer,
Tirumala Tirupathi
Devasthanams,
Hyderabad
2
Principal
Ashoka Institute of engineering and
Technology
3, 4
Jawaharlal Nehru Technological University, College of Engineering, Hyderabad, Andhra Pradesh,
Abstract:
In the present
experimental investigation
an attempt is made to report relationship between
compressive
strength , Split tensile Strength and Flexural Strength of High Strength Self Compacting Concrete
with mineral admixtures . It is well known that the properties of con
crete are affected by
cementitious matrix,
aggregate and the transition zone between the two phases. Reducing water powder ratio and addition of
pozollona admixtures like Fly ash
and Micro
silica are often used to modify the micro structure of the matrix
a
nd to optimize the transition zone.
Keywords:
Self Compacting Concrete, Segregation Resistance, Filling ability, Passing Ability, Water

Powder
Ratio.
I.
LITERATURE REVIEW
C.
SELVAMONY
et.al
(
1)
involved evaluating the Effectiveness of various percentages of mineral
admixtures in producing SCC. Okamura's method, based on EFNARC specifications, was adopted for mixed
design.
DRSRIRAVINDRARAJAHet.al
(
2
)
investigated
into the development of self

comp
acting concrete with
reduced segregation potential. The fine particle content is increased by replacing partially the fine and coarse
aggregates by low

calcium fly ash. S. VENKATESWARA RAO et.al
(3)
aims at developing standard and high
strength Self Compact
ing Concrete (SCC) with different sizes of aggregate based on Nansu’s mix design
procedure. Also, fly ash optimization is done in study with the graded coarse aggregate.
OKAMURA
(
4
)
proposed a mix design method for SCC based on paste and mortar studies for
super plasticizer
compatibility
followed by trail mixes. However, it is emphasized that the need to test the final product for passing ability,
filling ability, and flow and segregation resistance is more relevant
.
DR.SRINIVASA RAO. P
(
5
)
had proposed
the
relationship
between Splitting Tensile Strength and Compressive Strength by the test results and found that
Split Tensile Strength is proportional to 0.78 power of Compressive Strength for normal concrete.
DR.
SESHADRI SEKHAR .T
. P
6
)
had proposed the mix design for high strength self compacting concrete of
M100 mix using fly ash and Micro silica as Mineral admixtures .
DR SESHADRI
S
EKHAR .T
(
7
)
had proposed
the relationship between Compressive Strength , Flexural strength and Splitti
ng Tensile Strength for self
compacting concrete mix of different grades ranging from M30 to M65.
NIHAL ARIOGLU ET.AL
(8)
had
studied ratio of split tensile strength to cylinder compressive strength as a function compression strength of
concrete
.
Research
Significance
In fact, concrete researchers have shown that the true tensile strength, as determined from the split
cylinder test, is between 65 and 75 per cent of the modulus of rupture
for normal concrete
. It has been well
established that the splitting
tensile test of the cylindrical specimen gives more reasonable tensile strength
estimation than the direct tensile test or the modules of rupture test. The acceptance of the split cylinder test is
based on the fact that the stress distribution is reasonabl
y uniform along the vertical diameter of the cylinder,
which has been shown to be the plane of principle tensile stress for about 80 per cent of its length.
In a number of recent investigations of the behaviour of actual concrete dams during earthquakes, i
t has become
apparent that a limiting factor has been that the tensile strength of any concrete is only a fraction of its
American Journal of Engineering Research (AJER)
201
3
w w w.a j e r.u s
w w w.a j e r.u s
Page
68
Page
68
compressive strength. However, ACI building code provisions are primarily based on tests of relatively mature
concrete elements, and p
rovisions may not provide consistent safety margins when applied to young concrete. In
ACI, such strengths as modulus of rupture, shear, and splitting tensile strength of concrete are expressed in
terms of the square root of the compressive strength. These
empirical relationships were derived from tests on
relatively mature concrete specimens, and the square root function was probably chosen as a matter of
convenience so that calculations could be readily performed with a slide rule. However, recent researc
h has
shown that a square root relationship between splitting tensile strength and compressive strength is not the most
appropriate relationship for maturing concrete. It is evident that most concrete researchers believe, from
analyses of test data that th
e true test data is representative of power relation, which lies between 0.6 and
0.8.
For a newly development material like Self Compacting Concrete studies on Compressive, Split
Tensile and Flexural strength are of paramount important for instilling confi
dence amongst the engineers and
builders. The
literature indicates
that while some
studies are
available on the Compressive
Strength
, Split
Tensile
Strength
and Flexural Strength of Self Compacting
Concrete. Comprehension studies
which involve
relationship
between the parameters
Compressive
Strength
, Split Tensile
Strength
, Flexural Strength are not
available
High
Strength Self
Compacting Concrete
Mixes.
Hence, considering the gap in the existing
literature,
an attempt also has been made to obtain a relatio
nship between the splitting tensile strength, Flexural Strength
and Compressive
strength.
Experimental Programme
The objectives of the experimental study that was conducted are given below.
(i)
To develop Mathematical Relationship between Compressive
Strength, Split Tensile Strength and Flexural
Strength.
II.
MATERIALS
Cement
Ordinary Portland cement of 53 grade having specific gravity was
3.02
and fineness was 3200cm
2
/gm was used
in the investigation. The Cement used has been tested for various
proportions as per IS 4031

1988 and found to
be confirming to various specifications of are 12269

1987.
Coarse Aggregate
Crushed angular granite metal of 10 mm size having
the specific
gravity of 2.65 and fineness modulus 6.05 was
used
in the investigatio
n
.
Fine Aggregate
River sand having
the specific
gravity of 2.55 and fineness modulus 2.77 was used in the investigation.
Viscosity Modifying Agent
A Viscosity modified admixture for Rheodynamic Concrete which is colourless
free flowing liquid and having
Specific of gravity 1.01
+
0.01 @ 25
0
C and pH value as 8
+
1 and Chloride Content nil was used as Viscosity
Modifying Agent
.
Admixture
The Modified Polycarboxylated Ether (BASF Glenium
TM
B276 SURETEC) based
super plasticizer
wh
ich is
pale yellow colour and free flowing liquid and having Relative density 1.10
+
0.01 at 25
o
C, pH >6 and Chloride
Ion content <0.2% was used as
super plasticizer
.
Fly Ash
Type

II fly ash confirming to
I.S. 3812
–
1981of Indian Standard
Specification was
used as Pozzolana
Admixture.
Micro Silica
The Micro silica having the specific gravity
2.2 obtained
from Oriental Trexim, Private Limited was
used in the present investigation
Test Specimens:
Test specimens consist of 150X150X150 mm cubes, 150 X 300 mm cylinders and 100X100X 500 mm beams
were casted
for Mix
100
and tested as per IS 516 and 1199.
American Journal of Engineering Research (AJER)
201
3
w w w.a j e r.u s
w w w.a j e r.u s
Page
69
Page
69
III.
DISCUSSION OF RESULTS
Quantities of materials required per 1 cum
of High
Strength Self
Compacting
Concrete mixes
Table 1.0 gives the quantities of material required for High Strength Self Compacting mix
of grade M 100.
The
Trail Mixes were carried by verifying the fresh state properties with EFNARC guidelines.
Fresh State properties
of High
Strength Self
Compacting Concrete mixes
Table
2.0 provides
a summary of the fresh state
properties of
High
Strength Self
Compacting
Concrete
of
Mix 100.
As it is evident, the basic requirements of high
flow ability
and segregation resistance as specified
by guidelines on
High
Strength Self
Compacting Concrete mixes
by EFNARC are satisfied. The
Rheological
properties are maintained by adding suitable quantities of super
plasticizers which
satisfies
the
EFNARC
(
8
)
guidelines.
Mathematical Relationship
Betweeen Mechanical Properties
o
f High Strength
Self Compacting Concrete
Mix M 100
Table
3.0
gives the Compressive Strength , Flexural strength and Split Tensile Strength of M 100 grade
of High Strength Self Compacting Concrete for 7, 28, 56
,
90
, 180 and
270 days
. Based on the results of the
specimens the mathematical
equations were
obtained expressing Compressive Strength, Split Tensile Strength
and Flexural Strength for
High Strength Self Compacting Concrete
of
Mix M
100.
Fig
1
.0
shows the
graphical
behaviour of Compressive Strength
and Split
Tensile
Strength,
fig
2
.0 shows
the graphical
behaviour of
Compressive Strength
and Flexural
strength.
The mathematical relationship between both
between Compressive
Strength
–
Split Tensile Strength and Compress
ive Strength
–
Flexural Strength of Self Compacted Concrete
depicts that they
are obeying
Power Law.
Plate no 1, 2 and 3 gives the test setup for measuring Compressive
Strength, Split tensile Strength and Flexural Strength.
The Relationship between Compre
ssive Strength
–
Split Tensile Strength is given by
ft
= 0.04
3
f
c
k
1.0
6
4
with
coefficient of variation
R² = 0.9
90
The Relationship between Compressive Strength
–
Flexural Strength is given by
fcr
=0.0
3
1
fck
1.
125
with
coefficient of variation
R² = 0.98
9
IV.
CONCLUSIONS
The Relationship between Compressive Strength
–
Split Tensile Strength is given by
ft= 0.043fck
1.064
with
coefficient of variation R² = 0.990
The Relationship between Compressive Strength
–
Flexural Strength is given by
fcr=0.03
1
fck
1
.125
with
coefficient of variation
R² = 0.98
9
The Relationship between Compressive, Split Tensile and Flexural Strength
of High Strength Self
Compacting
C
oncrete are
in
accordance with power’s law.
The Water
–
Powder Ratio of .022 is used for getting High Strength Self Compacting Concrete of Mix M
100.
REFERRENCES
[1].
Selvamony C
et.al.
., “Development of high strength self compacted self curing concrete with mineral admixtures” International
Journal Design
and manufacturing
Technologies, Vol.3, No.2, July 2009,pp 103

108.
[2].
Dr. R. Sri Ravindrarajah,
et.al
“Development of high strength sel
f compacting concrete with reduced segregation potential
”
Proceedings of the 3rd International RILEM
Symposium,
Reykjavik, Iceland, 17

20 August 2003, Edited by O. Wallevik and I.
Nielsson , (RILEM Publications), 1 Vol., 1048 pp., ISBN: 2

912143

42

X, soft
cover.
[3].
S. Venkateswara Rao
et.al”
Effect of Size of Aggregate and Fines on Standard And High Strength Self Compacting Concrete”,
Journal of Applied Sciences Research, 6(5): 433

442, 2010.
[4].
Hajime Okamura
et.al
,
”
Self Compacting Concrete”, Journal of Advan
ced Concrete Technology,Vol 1, No 1,5

15, April 2003.
[5].
Dr.P.Srinivasa Rao
et.al “Relationship
between
Splitting
Tensile and Compressive Strength of Concrete
”,
Construction Review
Journal June, 39

44.
[6].
Dr T. Seshadri
Sekhar et.al
“High Strength self compa
cting concrete using mineral admixtures ” , Indian Concrete Journal March
2013 PP 42

48.
[7].
7
.
Dr T. Seshadri Sekhar
et.al
“Relationship between Compressive, Split Tensile, Flexural Strength of Self Compacting
Concrete” publication in Internation
al Journal of Mechanics and Solids, Volume 3, Number 2 (2008) pp 157

168.
[8].
EFNARK, “
Specifications and guidelines for self compacting concrete
”,
www.efnarc.org
American Journal of Engineering Research (AJER)
201
3
w w w.a j e r.u s
w w w.a j e r.u s
Page
70
Page
70
0
1
2
3
4
5
6
7
8
9
10
0
50
100
150
200
Split Tensile Strength (Mpa)
Compressive Strength (Mpa)
Fig 1.0 Relationship between Compressive Strength and Split Tensile
Strength
American Journal of Engineering Research (AJER)
201
3
w w w.a j e r.u s
w w w.a j e r.u s
Page
71
Page
71
Plate No1 Test Set up for measuring
Plate No2 Test Set up
for measuring
Compressive Strength
Flexural Strength
Plate No3 Test Set up for measuring Split Tensile Strength
0
1
2
3
4
5
6
7
8
9
10
0
20
40
60
80
100
120
140
160
Flexural Strength (MPa)
Compressive Strength (MPa)
Fig 2.0 Relationship between Compressive Strength and Flexural Strength
Σχόλια 0
Συνδεθείτε για να κοινοποιήσετε σχόλιο